h i g h l i g h t s
he therngs incwith wm corred on th
experimental results show that the lightening of concrete by wood shavingslation capacity by decreasing the thermal conductivity and diffusivity; how-
The composite woodconcrete has been studied a lot these last
wood bers are naturally degradable , which is not negligible inthe current context of waste limitation. The reinforcement of con-crete by wood bers gives a composite material which can be usedin many applications such as oor formwork, suspended ceilings,screeds and interior masonry blocks .
Several studies have focused on the use of wood as ash in con-crete . Based on its physical, chemical, and microstructural
products, roller-compacted concrete pavements (RCCPs), materialst al.  study theexaminincture. The
are encouraging and indicate the feasibility of producing aweight concrete. Bederina and Quneudec , Ziregue [8that the addition of wood shavings in concrete improves itmal insulation performance, while decreasing its compressivestrength. However, it is possible to ensure a compromise betweenthe compressive strength and the thermal conductivity for obtain-ing a structural insulation concrete.
Nevertheless, this material can present a high hygroscopicbehavior due to the strong absorption of wood particles. When thismaterial has being exposed to the conditions of temperature (T)and relative humidity (RH), which are variable between the interior
Corresponding author. Tel.: +212 0667540261.
Construction and Building Materials 48 (2013) 104115
Contents lists available at
evE-mail address: firstname.lastname@example.org (D. Taoukil).years because wood bers have many advantages: low cost,healthier production processes for the production of compositeswith different forms, the renewal and the recycling . In addition,
for road base, and blended cements. Coatanlem edurability of wood chipping concrete mixture bypressive strength, exural strength and microstru0950-0618/$ - see front matter 2013 Elsevier Ltd. All rights reserved.http://dx.doi.org/10.1016/j.conbuildmat.2013.06.067g com-resultslight-
] shows ther-Keywords:Wood concreteThermal conductivityThermal diffusivityMoisture contentHygrothermal effect
ever these proprieties are strongly dependent on water content. The thermal conductivity increasesrapidly with water content. Its experimental evolution with water content was conrmed by the com-parison with three theoretical models. The values of the thermal diffusivity depend on the used count-ing model. The results stemming from three most used models are compared between them, and theyshow that in general the thermal diffusivity presents a maximum corresponding to a water contentvalue Wm.
2013 Elsevier Ltd. All rights reserved.
1. Introduction properties, the authors reported that wood ash has a signicant po-tential for use in low and medium strength concrete, masonryAvailable online 23 July 2013been examined herein. Theincreases the thermal insu The inuence of moisture content on t Lightening the concrete by wood shavi Thermal conductivity increases rapidly Thermal diffusivity presents a maximu The values of thermal diffusivity depen
a r t i c l e i n f o
Article history:Received 29 November 2012Received in revised form 30 May 2013Accepted 17 June 2013mal proprieties of woodconcrete is studied.reases its thermal insulation capacity.ater content.sponding to a water content value Wm.e used counting model.
a b s t r a c t
The aim of the work reported in this paper is to determine the inuence of moisture content on thethermal proprieties of woodconcrete composite, i.e. thermal conductivity and thermal diffusivity.The wood shavings have been incorporated, without any preliminary treatment, into a sandcementmixture. Five formulations containing different percentage of shavings have been prepared and haveHTW Berlin, University of Applied Sciences, Ingenieurwissenschaften I, Berlin, GermanyMoisture content inuence on the thermof woodconcrete composite
Driss Taoukil a,, Abdelmajid El bouardi a, Friedrich Sia Energetic Laboratory, Physics Department, Faculty of Sciences of Tetuan, Abdelmalek E
journal homepage: www.elsconductivity and diffusivity
b, Abdelaziz Mimet a, Hassan Ezbakhe a, Taib Ajzoul a
di University, Morocco
ier .com/locate /conbui ldmat
and the exterior of the building, heat and moisture transfers occurwithin the medium. An important interaction develops betweenthe heat and the moisture transfers and the different transportproperties . Indeed, the thermal, phonic and mechanical proper-ties of the material are modied. It is thus crucial to quantify thevariation of these properties with temperature and moisture con-tent of the sample. But, this is not considered in most studies treat-ing the use of this type of material in building. In this context, thisstudy has been conducted to measure the effect of moisture con-tent on the thermal conductivity and diffusivity of the woodconcrete composite.
2.1. Basic materials
The wood shavings used are a sawmill waste (Fig. 1). They correspond to thespecies generally used in the carpentry work in Morocco . The granulometricanalysis by sieving, established by a method identical to that proposed by theFrench standard NF P18-560 , demonstrates that the used wood shavings havea particle size between 8 mm and 20 mm. The sand is sea one of granulometry 0/5and of bulk density on the order of 1500 kg/m3. This sand is used without any wash-ing procedure. Indeed, the test of sand equivalent made according to the standardNF EN 933-8  gives the value 81%, which shows that it is a clean sand with a
The constituents are mixed in a mixer at slow speed on the order of 50 r min1,
models used in this work are as follows:
3.1. Krischer and Kroll model 
The Krischer and Kroll model is a combination between the se-rial and the parallel models. The authors suppose that the volumefraction h of layers oriented perpendicular to the direction of heatow is arranged in series with the complementary fraction (1h) oflayers oriented parallel to the direction of heat ow. Firstly, theauthors suppose that the uid phase consists only of gas (air ingeneral). Afterwards, they extend their model for a uid phase con-sisting of gas and liquid (water in general). The apparent thermalconductivity is given by a harmonic mean of the series and parallelmodels:
D. Taoukil et al. / Construction and Buildin order to obtain a good homogenization of the components. The durations of thedifferent phases of mixing must be sufciently long to allow a good homogenizationand short enough to avoid leaving too much water to evaporate in ambient air.Thus, three phases are distinguished:
Mixing cement and sand: 3 min. Adding pre-wetted wood shavings: 3 min. Adding mixing water and mixing: 5 min.low percentage of clay nes, suiting perfectly for high quality concretes . Thecement used is Portland cement CPJ 35 equivalent to CEM II 22.5 and whose tech-nical characteristics are in accordance with the Moroccan standard NM 10.01.004. The used mixing water is a tap water.
The concretes prepared are based on a mass ratio of 2/3 of sand and 1/3 of ce-ment. The specimens are made with a mass ratio of water to cement (W/C) of 0.6.The study was conducted on ve formulations containing different proportions ofwood shavings.
2.2. Implementation of fresh concreteFig. 1. General aspect of the used wood shavings.2.3. Preparation of specimens
The homogenized mixture is then introduced into parallelepiped molds; twodimensions of molds were made according to the type of tests to be realized. As re-gards the thermal aspects, the molds of dimension (27 27 2 cm3) were used. Formechanical strength, the molds (16 4 4 cm3) were used. These different sizesare related to measuring devices (thermal box, mechanical press) whose dimen-sions are imposed. The use of the same manufacturing process, regardless of themold, allows to work on the same material.
The specimens are preserved before and after turning out into the room test at acontrolled temperature and humidity (Ta = 20 C, RH = 60%). These conditions corre-spond to a standard climate and allow to reproduce real conditions of the use of thematerial.
The elaborate formulations, containing various rations in wood shavings, arepresented with their physico-mechanical properties in Table 1.
The density and the porosity are strongly inuenced by the addition of woodshavings. Thus, a progressive decrease in density and an increase in porosity are ob-served. Indeed, the sand concrete, due to its small granularity, is lighter than ordin-ary concrete. The introduction of wood shavings reduces it more. The higher theproportion of wood shavings used the lighter the sand concrete will be [7,16,17].This lightness is due, on the one hand, to the porous structure of wood, on the otherhand, to an additional porosity led in the matrix when the water absorbed by thewood shavings evaporates during the drying.
The increase in shavings content reduces the mechanical strength of concrete.This decrease is due, on the one hand, to the low mechanical strength of the inclu-sions, and on the other hand, to the increase of porosity.
The water absorption capacity is very sensitive to the addition of wood shav-ings. Thus, there is a signicant increase in Wsat. Indeed, wood particles have a verymarked brous aspect. The canals which lead the sap give this material a highporosity communicating via orices. This leads to a strong hygroscopic character. It is noted that the concrete sand, itself, is characterized